Originally approved in Last previous edition approved in as E–99 DOI: /E 2 For referenced ASTM standards. ASTM E()e1. Standard Practice for Microetching Metals and Alloys. standard by ASTM International, 06/01/ View all product details. Determination of Residual Stresses Numerically Obtained in ASTM AH36 Steel Welded by TIG Process. Pablo Batista Guimarães, Paulo.
|Published (Last):||12 March 2009|
|PDF File Size:||18.81 Mb|
|ePub File Size:||3.45 Mb|
|Price:||Free* [*Free Regsitration Required]|
Add the HCl just before using. Swab until stain is removed.
This is imperative with etchants that give off noxious e47 or toxic vapors that may accumulate or become explosive. If pitting occurs, reduce voltage. Swab 1—3 s for F and T6, 10 s for Atm and O temper. Repeat three times and repolish lightly.
Electrolytic at 80 V for 5—30 min. This standard has been approved for use by agencies of the Department of Defense. Will chemically polish with longer times. Reveals Ti- and Cb-rich areas at a faster rate than grain boundaries. See Guide E on Metallographic Laboratory Safety for additional information on safety precautions for electrolytes containing perchloric acid. Alloys are listed as a group or series when astk or more etchants are common to the group or series.
Swab gently 10—15 s.
Electrolytic at 60— V for 5—30 s. All persons using any etchants should be thoroughly familiar with all of the chemicals involved and the proper procedure for handling, mixing, and disposing of each chemical, as well as any combinations of those chemicals. Continued Procedure Use a certi? The HF may be varied to give more or less etching.
ASTM E – 07()e1 Standard Practice for Microetching Metals and Alloys
Pure Ta Ta alloys, 62 65, 61, 62, 66,general general general general general structure structure structure structure structure general structure general structure grain boundaries and inclusions grain boundaries—retains carbide precipitate Thorium Base: Electrolytic at 6 V for 5—10 s.
Electrolytic astn 6 V for few seconds to a minute. A superscript epsilon e indicates an editorial change since the last revision or reapproval. A mixture of 5 drops of each will cover the surface of a 1 in.
For best results use before pellets have dissolved. Immerse in Solution A with gentle agitation for several seconds. Buying HF at the lowest useable concentration will signi? Immerse specimen face up.
Precaution—Also poisonous by ingestion as well as skin contact. The specimen is placed in the solution using tongs, polished face up. Activity may be decreased by substituting glycerol for water. Mix equal volumes of Solutions A and B just before use.
E4077 standard is subject to revision at asfm time by the responsible technical committee and must be reviewed every? Swab for 1—3 min. Immerse with gentle agitation 15—30 s. Experience has shown that the quality of tap water varies signi? Properly discard Solution B after 1 hr. Electrolytic at 30 V for 30 s. Summary of Practice 4.
When more than one etchant number is given for a particular use, they are usually given in order e47 preference. Colors phosphides in cast iron. Immerse with gentle agitation 5—15 s.
ASTM E407-07 Standard Practice for Microetching Metals and Alloys
Excellent grain boundary etch for ferritic stainless steels. Repeat as often as necessary. A vacuum level of 1.